Inverted organic photovoltaic device with a new electron transport layer
© Kim et al.; licensee Springer. 2014
Received: 13 February 2014
Accepted: 18 March 2014
Published: 27 March 2014
We demonstrate that there is a new solution-processed electron transport layer, lithium-doped zinc oxide (LZO), with high-performance inverted organic photovoltaic device. The device exhibits a fill factor of 68.58%, an open circuit voltage of 0.86 V, a short-circuit current density of −9.35 cm/mA2 along with 5.49% power conversion efficiency. In addition, we studied the performance of blend ratio dependence on inverted organic photovoltaics. Our device also demonstrates a long stability shelf life over 4 weeks in air.
KeywordsLithium Zinc oxide Organic photovoltaic Stability Solution-processed Electron transport layer Blend ratio
Next-generation organic photovoltaics (OPVs) require not only semiconductors with high performance, but also for them to feature high optical transparency, low temperature, and solution processability. Currently, metal oxide interlayers are widely used as hole and electron buffer layers in OPVs. However, OPVs have relatively low energy efficiency (12%) , and their deposition requires a costly vacuum deposition technique. Accordingly, in a search for an alternative for metal oxide interlayer, considerable attention has been given to metal oxide semiconductor, such as indium zinc oxide (IZO) [1–5], zinc oxide (ZnO) [6–10], aluminum-doped zinc oxide (AZO) [11–15], titanium oxide (TiO x ) [16–20], graphene oxide (GO) [21–25], tungsten oxide (WO x ) [26–30], nickel oxide (NiO x ) [31–35], molybdenum oxide (MoO x ) [36–40], vanadium pentoxide (V2O5) [41–45], and reduced graphene oxide (rGO) [46–50], as these oxides have high optical transparencies, excellent electrical properties, chemical stability, and solution processability. For instance, TiO x -based semiconductors have been successfully employed in various electronic devices, namely, as an electron transport layer for solar cells, energy harvesting devices with piezoelectric properties, and channel materials for thin film transistor (TFT). In OPVs, TiO x [20–25] films are deposited using various techniques, such as chemical bath deposition, spray pyrolysis, and rf magnetron sputtering. Although sputtering and vapor deposition methods have ensured high device performance and reliability, they are costly and the procedure is cumbersome. Nonetheless, solution processing of TiO x allows large-area and low-cost manufacturing. However, it compromises the resulting energy efficiency as well as carrier mobility.
Thus, various zinc oxides such as IZO [6–10] which has good solution processability at relatively low temperature have been introduced. However, in spite of their good performance, we are now running out of indium supply. The price of indium has increased in the last 10 years, and indium has become increasingly scarce. Therefore, to resolve these problems, indium-free ZnO-based semiconductor has been introduced. Because these methods were based on a sol-gel process with hydrocarbon complexes, they all suffered from residual carbon impurities which hamper electron transfer. In order to remove the impurities, an annealing process must take place at a high temperature of at least 400°C. Furthermore, to improve the energy efficiency, the ZnO solution must be processed without the presence of indium compounds and carbon and must be processed at a low temperature. Recently, it is been reported that the carbon-free method at a low temperature can be processed and is compatible with mechanically flexible substrates. However, the electron mobility of ZnO as described in this study is inadequate for use in high-quality OPVs .
To overcome the aforementioned challenges, we adopted alkali metal dopants focusing particularly on lithium in order to fabricate solution-processed OPVs with enhanced energy efficiency and stability. We used lithium as a dopant because it has comparable conductivity (2.25 × 10−6 S/cm) compared to ZnO. According to literature, the cost of 100 g of bulk lithium is nearly US$10 . We introduced a unique aqueous PEDOT:PSS-doped carbon nanotube (CNT), which successfully created a new interface engineering as the buffer layer at maximum process temperature as low as 80°C for 30 min. Additionally, the influence of the dopant concentration on the device performance was also examined. Lithium-doped zinc oxide (LZO) OPVs demonstrated a maximum energy conversion efficiency of 5.49%, with a fill factor of 68.58%. Furthermore, LZO devices also exhibited excellent shelf life in an air test that lasted over 30 days.
LZO solution preparation
Zinc acetate dihydrate (99.9%, Merck, Gangnam-gu, Seoul, South Korea) was used as a starting material and was recrystallized twice from double distilled water. The complexes with monoethanolamine have been prepared in ethanol solution. Resultant complexes of 1:1 stoichiometric composition have been obtained . Lithium chloride was used as a doping agent in zinc-acetate-based precursors.
Patterned indium tin oxide (ITO)-coated glass with a sheet resistance of 15 Ω/sq was cleaned inside an ultrasonic bath. First, it was cleaned with deionized water, followed by acetone, methanol, 2-propanol, and finally with ultraviolet (UV) ozone. A ferroelectric solution-processed LZO solution was spin-coated (600 rpm) on the top of the ITO substrate and dried at 245°C for 10 min to form a thin interlayer of 35 nm. The thickness of the interlayer was determined following a previously published paper . The active layer (P3HT:ICBA = 1:1, 1.5 wt.%), with a thickness of 85 nm, was then coated on top of the interlayer, by casting from a dichlorobenzene solution and drying it at 150°C for 10 min. The thickness of the active layer was verified by a surface profilometer (Alpha-Step profilometer; KLA Tencor, Milpitas, CA, USA). The PEDOT:PSS:CNT was coated on the active layer at 4,000 rpm for 25 s and later annealed at 120°C for 20 min. Finally, a 100-nm aluminum layer was evaporated with a shadow mask. The overlapping area between the cathode and the anode defined the device active area of 0.04 cm2. All the fabrication processes were carried out inside a controlled atmosphere of a nitrogen drybox (mBRAUN, Stratham, NH, USA) containing less than 10 ppm oxygen and moisture.
J-V and EQE
The power conversion efficiencies of the inverted OPVs were measured under an illumination of AM1.5G simulated solar light (Oriel Model 91192; Oriel Instruments, Stratford, CT, USA) at 100 mW/cm2. The current density-voltage (J-V) characteristics were recorded with a Keithley 2410 source unit (Keithley Instruments Inc., Cleveland, OH, USA). The external quantum efficiency (EQE) measurements were performed using an EQE system (model 74000) obtained from Newport Oriel Instruments USA and Hamamatsu (Hamamatsu Photonics, Hamamatsu, Japan) calibrated silicon cell photodiode used as a reference diode. The wavelength was controlled with a monochromator at 200 to 1,600 nm.
Ultraviolet photoelectron spectroscopy
Ultraviolet photoelectron spectroscopy (UPS) measurements were performed using the He I photon line (hv = 21.22 eV) of a He discharge lamp under UHV conditions (4 × 10−10 mbar). Emitted photoelectrons were collected using a semi-spherical channeltron with analyzer pass energy set to 5 eV. XPS was carried out using a MgKα line (hv = 1,253.6 eV) with an analyzer pass energy of 10 eV.
Spectroscopy ellipsometry measurements were gathered using of a rotating analyzer Woollam variable angle spectroscopic ellipsometer (WVASE) system, equipped with a high-pressure Xe discharge lamp integrated in an HS-190 monochromator.
Atomic force microscopy
Atomic force microcopy (AFM) imaging was completed in air using digital instrument multimode equipped with a nanoscope IIIa controller.
Resistivity and Hall measurements
The measurement of Hall effect was carried out in Van der Pauw configuration with a constant current of 100 A using high-resolution instruments, with an accuracy of approximately 1.5%. Hall measurements were repeated for different magnetic fields and different applied voltages on the same sample.
Results and discussion
The energy-level diagram illustrating the highest occupied molecular orbital and lowest unoccupied molecular orbital (HOMO-LUMO) of all materials used in the inverted OPVs, together with the work functions of the electrodes, is shown in Figure 1c. In this device, the LZO buffer layer may function as (i) electron-transporting and a hole/or exciton-blocking layer and (ii) as a modifier of the ITO work function at the ITO/P3HT interface, whereas the PEDOT:PSS:CNT buffer layer serves as a barrier layer by preventing the diffusion of the Al cluster (due to thermal evaporation) from penetrating through the photoactive layer.
As shown in Figure 1c, the LUMO of CNT (1.6 eV) is much higher than the LUMO of either donor P3HT (3.2 eV) or acceptor (3.74 eV), showing that CNT can efficiently block the backflow electron from indene-C60 bisadduct (ICBA) to Al electrode. This has shown good hole extraction ability in combination with Al as the top anode in inverted OPVs. LZO possesses conduction and valance bands of 4.4 and 7.6 eV, respectively, and can block backflow holes. Since the HOMO and LUMO levels of P3HT are 5.2 and 3.2 eV, respectively, the HOMO level of P3HT is well aligned to the HOMO level of CNT, which can benefit the hole extraction. The work function of LZO is 4.6 eV, which is moderately aligned with that of ICBA and can supply good electron extraction from the ICBA acceptor phase. Interestingly, photovoltaic results in this work indicate that PEDOT:PSS:CNT could efficiently extract holes from the P3HT to the Al anode. It is understood that the LZO interlayer can supply good electron extraction from the ICBA acceptor because of their moderately aligned conduction band. However, the LUMO level of 3.4 eV of ICBA is almost 0.9 eV higher than that of LZO. This is a moderate energy barrier for electron transport. According to the photovoltaic performances of the LZO-based inverted OPVs, electrons should be efficiently collected by the ITO cathode, suggesting that the LZO must afford a necessary electron pathway.
Summarized key parameters of inverted organic photovoltaics with different LZO concentrations
(Ω cm −2 )
(Ω cm −2 )
(cm 2 V s)
The effect of LZO on the performance of OPVs is as follows: the complete inverted OPVs which consist of ITO/cathode buffer layer/P3HT:ICBA/anode buffer layer/Al structure were fabricated to study the electron buffer layer dependence, the EQE trends, current-voltage characteristics under AM1.5G (100 mW/cm2) solar-illuminated conditions, and device stability over 720 h. The blend ratio of the cathode buffer layer was changed from 0 to 30 wt.% by controlling the concentration of lithium.
The large PCE improvement of the LZO 2 wt.%-based inverted OPVs is due to the largely elevated Jsc and FF. The average PCE of four LZO-2 wt.%-based inverted OPVs was 5.31%, demonstrating that LZO is a promising cathode buffer layer for high Jsc and high-efficiency OPVs. It should be noted that the Voc of 0.86 V for LZO is the highest among all metal oxide electron extraction materials. Some metal oxides also demonstrate high Voc in OPVs; however, these metal oxides showed lower PCE than that of LZO OPV. As the weight percentage increases to 10 and 30, the efficiencies of both devices decrease to 5.25 and 4.95, respectively. This indicates that Li doping enhances electron transport through ZnO. However, increasing the amount of Li led to a decrease in energy efficiency, which implies that Li doping of ZnO beyond 2 wt.% hampers electron transport. Such a decrease in Jsc and FF is caused when a significant amount of impurity (Li) is added to a ZnO film. This actually generates a number of charge traps. Additionally, when the Jsc is not saturated, it decreases when increasing the blend ratio. This can be seen in the case of a typical P3HT:ICBA bulk heterojunction inverted OPVs. When analyzing J-V characteristics, the amount of absorbed photon reduces depending on the blend ratio. Nevertheless, the amount of internal series resistance and deactivated carriers in the inverted OPVs actually increases, owing to the short carrier diffusion length in organic semiconducting materials. Due to the fact that LZO possesses low carrier mobility (Table 1), the transport process of the photogenerated carriers to the electrode could be inefficient. Consequently, we see that the Jsc is reduced even if high blending ratio is employed in our cells. However, FF decreased because of internal series resistance involving a cathode buffer layer in the LZO system. As we can see from J-V curves from Figure 4a, the blend ratio of 2 wt.% of the cathode buffer layer is the optimal value to achieve the best efficiency. We argue that the improvements on energy efficiency are possible because of two distinct reasons. The primary reason is that introductions of alkali metal (Li) will basically n-type dope ZnO and secondly for efficient hole collection and in-plane conductivity of our OPVs. A theory predicts that the presence of Li in the ZnO matrix prefers the interstitial sites (electron donor) over substitutional sites (acceptor) and thus n-type dopes ZnO. Shallow donors were experimentally tested in regard to Li atoms on ZnO. This was previously analyzed based on electron paramagnetic resonance and electron nuclear double resonance experiments . Concordantly, we observed an increase in Voc, implying that adding Li beyond a certain amount creates a greater number of defects in the ZnO film rather than doping them. Because CNT is a mixture of p-doped nanotubes and metals, PEDOT:PSS is required to adjust the CNT work function for hole collection. At the same time, it must avoid any shorts in the device by having metallic nanotubes transport electrons from the ICBA network to the appropriate electrode. The charge transfer and transport processes can be understood from the energy level diagram depicted in Figure 1c. As discussed above, the Jsc is not saturated and decreases with the increase of the LZO blend ratio. In PEDOT:PSS:CNT-based devices, the inverted OPVs work at a higher blend ratio (30 wt.%). Although it seems like a higher blend ratio reduces the absorbed photon, the transport process in the PEDOT:PSS:CNT-based devices seems to be efficient. This is also evident because it is resistive of the inverted OPVs, where the series resistance of 2, 10, and 30 wt.% is 13.91, 15.28, 17.07 Ω cm−2, respectively. Series resistance (Rs) and shunt resistance (Rsh) values for the inverted OPVs are also listed in Table 1. The Rs of the (LZO 2 wt.%) PEDOT:PSS:CNT-based OPVs was the smallest, and the other two devices did not show too much Rs difference. The Rsh values of the PEDOT:PSS:CNT-based OPVs were obviously smaller.
The EQEs of inverted OPVs with LZO and PEDOT:PSS:CNT-based devices (Figure 4b) show a slightly lower EQEmax of 64% at 520 nm (LZO 2 wt.%). The EQE curve is similar to that of the LZO 10 and 30 wt.%-based OPVs. For LZO 10 and 30 wt.%, the EQE values are about 63.4% and 59.3%, respectively. The integration of the EQE curves for LZO 2, 10, and 30 wt.% is in agreement with the Jsc values obtained from J-V characteristics (9.30, 8.93, and 8.55 mA/cm2, respectively).
According to literature, ZnO-based inverted OPVs have demonstrated good results of shelf life in air [6–10]. In this study, in the shelf life test in air of inverted OPVs with LZO as the interlayer, two inverted OPVs with different anode buffer layers were compared. In order to protect the top Al electrodes of OPVs, we covered the active layer of each device with a glass plate with UV glue in a N2 glovebox. After 1 min of UV curing, the devices were placed in air under ambient conditions for stability testing. Therefore, we used PEDOT:PSS:CNT as the interlayer on active layer to construct an inverted OPVs. This provided a promising shelf life test in air. It may be expected that using a more stable metal (Ag or Au) to replace Al as the top anode in the inverted OPVs would improve the shelf life test in air.
The stability of the inverted OPVs was measured over a period of 30 days. J-V and EQE characteristics for PEDOT:PSS:CNT devices were recorded in the mentioned time interval. The photovoltaic parameters were derived as a function of the degradation time (expressed in week), as tabulated in Additional file 1: Table S1. The PEDOT:PSS:CNT devices (Figure 4c,d,e) demonstrate significant results in the shelf life test in air during the first 2 weeks. Later, results start to decrease. However, results are still higher by nearly 4% even after being in storage for 4 weeks. The increased efficiency of PEDOT:PSS:CNT devices is due to a slight increase of Jsc and FF values in time. This can be attributed to improved charge transport and electron collection phenomena. We can speculate that the solution-processed LZO film becomes more crystalline over time. Thus, charge transport properties improve due to the inherent dimeric structure of the LZO in its crystalline form. While Jsc increases, Voc remains constant for almost the total period of stability measurements. The improvement of all the photovoltaic parameters for PEDOT:PSS:CNT devices indicates that the PEDOT:PSS:CNT buffer layer can prevent the diffusion of oxygen or vapor to the photoactive layer (P3HT:ICBA). The reproducibility of the described degradation trends was verified by investigating several identical devices. The corresponding EQE spectra are in agreement with the J-V characteristics (Additional file 2: Figure S1).
In spite of the moderate efficiencies demonstrated by the present devices compared to the highest state-of-the-art OPVs, their long-term durability and reliability in air is an interesting feature that should be further investigated. Based on our studies, the introduction of the LZO and PEDOT:PSS:CNT buffer layers is the key factor to achieving more stable cells. Thus, the LZO is a very interesting class of compound for the development of stable and efficient OPVs.
The newly synthesized LZO has been investigated as an electron buffer layer in P3HT:ICBA-based inverted OPVs with Al as the top electrode. The performance of the fabricated OPVs has been compared to that of similar devices containing a typical PEDOT:PSS:CNT hole buffer layer between the active layer and Al top electrode. LZO and PEDOT:PSS:CNT cells have higher efficiencies, excellent electron and hole transports properties, efficient electron/hole/exciton blocking properties, better energy alignment at the LZO/ITO interface, and increased cathode work function compared to ITO. In addition, LZO is believed to donate holes/energy to P3HT, which is also beneficial for the device performance.
LZO and PEDOT:PSS:CNT performance was enhanced to up 20%, indicating the most interesting compound for future use. The combination of LZO and PEDOT:PSS:CNT is the most promising for achieving efficient devices. Up to 20% of improvement in PCE was observed with respect to a device containing a GO buffer layer.
The stability of the devices has been accurately studied over 30 days. In spite of the exposure to open air during the whole measurements, the stability and reliability of the OPVs is excellent. In all cases, no significant loss of performance can be observed. The buffer layer effectively blocks the diffusion of oxygen and vapor through the photoactive layers, which has a detrimental effect on the cell stability. Devices containing PEDOT:PSS:CNT are stable, and after 30 days their efficiencies is still close to their initial values.
The key role of LZO and PEDOT:PSS:CNT in the enhancement of the cell efficiency and stability suggests the use of this class of compounds as an alternative to other widely known buffer materials. The presented results could be applied to more advanced and highly efficient devices as well, combining the advantages of high performance with the long stability. This is ensured by the introduction of LZO and PEDOT:PSS:CNT buffer layers.
This work was supported by the Industrial Strategic Technology Development (10045269, Development of Soluble TFT and Pixel Formation Materials/Process Technologies for AMOLED TV) funded by MOTIE/KEIT.
- Puetz A, Steiner F, Mescher J, Reinhard M, Christ N, Kutsarov D, Kalt H, Lemmer U, Colsmann A: Solution processable, precursor based zinc oxide buffer layers for 4.5% efficient organic tandem solar cells. Org Electron 2012, 13: 2696. 10.1016/j.orgel.2012.07.043View Article
- Zheng Q, Fang G, Cheng F, Lei H, Wang W, Qin P, Zhou H: Hybrid graphene/ZnO nanocomposites as electron acceptor in polymer-based bulk-heterojunction organic photovoltaics. J Phys D Appl Phys 2012, 45: 455103. 10.1088/0022-3727/45/45/455103View Article
- Ma Z, Tang Z, Wang E, Andersson MR, Inganäs O, Zhang F: Influences of surface roughness of ZnO electron transport layer on the photovoltaic performance of organic inverted solar cells. J Phys Chem C 2012, 116: 24462. 10.1021/jp308480uView Article
- Kim HP, Ryu MS, Youn JH, Yusoff ARBM, Jang J: Photomask effect in organic solar cells with ZnO cathode buffer layer. IEEE Electron Device Lett 2012, 33: 1480.View Article
- Keian N, Giustino F: Ideal energy-level alignment at the ZnO/P3HT photovoltaic interface. Adv Funct Mater 2012, 22: 5089. 10.1002/adfm.201201478View Article
- Kyaw AKK, Wang Y, Zhao DW, Huang ZH, Zeng XT, Sun XW: The properties of sol-gel processed indium-doped zinc oxide semiconductor film and its application in organic solar cells. Phys Status Solid A 2011, 208: 2635. 10.1002/pssa.201127263View Article
- Choa SH, Cho CK, Hwang WJ, Eun KT, Kim HK: Mechanical integrity of flexible InZnO/Ag/InZnO multilayer electrodes grown by continuous roll-to-roll sputtering. Sol Energy Mater Sol Cells 2011, 95: 3442. 10.1016/j.solmat.2011.08.001View Article
- Chen X, Taguchi D, Manaka T, Iwamoto M: Analyzing photo-induced interfacial charging in IZO/pentacene/C60/bathocuproine/Al organic solar cells by electric-field-induced optical second-harmonic generation measurement. J Appl Phys 2012, 111: 113711. 10.1063/1.4728225View Article
- Besleaga C, Ion L, Ghenescu V, Socol G, Radu A, Arghir I, Florica C, Antohe S: Transparent indium zinc oxide thin films used in photovoltaic cells based on polymer blends. Thin Sol Film 2012, 520: 6803. 10.1016/j.tsf.2012.07.030View Article
- Kim HP, Yusoff ARBM, Ryu MS, Jang J: Semi-transparent organic inverted photovoltaic cells with solution processed top electrode. Org Electron 2012, 13: 3195. 10.1016/j.orgel.2012.09.012View Article
- Hayashi H, Lightcap IV, Tsujimoto M, Takano M, Umeyama T, Kamat PV, Imahori H: Electron transfer cascade by organic/inorganic ternary composites of porphyrin, zinc oxide nanoparticles, and reduced graphene oxide on a tin oxide electrode that exhibits efficient photocurrent generation. J Am Chem Soc 2011, 133: 7684. 10.1021/ja201813nView Article
- Yang K, Xu C, Huang L, Zou L, Wang H: Hybrid nanostructure heterojunction solar cells fabricated using vertically aligned ZnO nanotubes grown on reduced graphene oxide. Nanotechnology 2011, 22: 405401. 10.1088/0957-4484/22/40/405401View Article
- Yun JM, Yeo JS, Kim J, Jeong HG, Kim DY, Noh YJ, Kim SS, Ku BC, Na SI: Solution-processable reduced graphene oxide as a novel alternative to PEDOT:PSS hole transport layers for highly efficient and stable polymer solar cells. Adv Mater 2011, 23: 4923. 10.1002/adma.201102207View Article
- Jeon YJ, Yun JM, Kim DY, Na SI, Kim SS: High-performance polymer solar cells with moderately reduced graphene oxide as an efficient hole transporting layer. Sol Energy Mater Sol Cells 2012, 105: 96.View Article
- Yusoff ARBM, Kim HP, Jang J: Solution processed encapsulation for organic photovoltaics. Sol Energy Mater Sol Cells 2013, 110: 87.View Article
- Zilberberg K, Trost S, Meyer J, Kahn A, Behrendt A, Hecht DL, Frahm R, Riedl T: Inverted organic solar cells with sol-gel processed high work-function vanadium oxide hole-extraction layers. Adv Funct Mater 2011, 21: 4776. 10.1002/adfm.201101402View Article
- Shen L, Ruan S, Guo W, Meng F, Chen W: Semitransparent inverted polymer solar cells using MoO3/Ag/V2O5 as transparent anodes. Sol Energy Mater Sol Cells 2012, 97: 59.View Article
- Gong C, Yang HB, Song QL, Li CM: Nanostructure effect of V2O5 buffer layer on performance of polymer-fullerene devices. Org Electron 2012, 13: 7. 10.1016/j.orgel.2011.10.006View Article
- Wang HQ, Li N, Guldal NS, Brabec CJ: Nanocrystal V2O5 thin film as hole-extraction layer in normal architecture organic solar cells. Org Electron 2012, 13: 3014. 10.1016/j.orgel.2012.08.007View Article
- Yusoff ARBM, Kim HP, Jang J: Inverted organic solar cells with TiOx cathode and graphene oxide anode buffer layers. Sol Energy Mater Sol Cells 2013, 109: 63.View Article
- Chen L, Wang P, Li F, Yu S, Chen Y: Efficient bulk heterojunction polymer solar cells using PEDOT/PSS doped with solution-processed MoO3 as anode buffer layer. Sol Energy Mater Sol Cells 2012, 102: 66.View Article
- Wong KH, Ananthanarayanan K, Luther J, Balaya P: Origin of hole selectivity and the role of defects in low-temperature solution-processed molybdenum oxide interfacial layer for organic solar cells. J Phys Chem C 2012, 116: 16346. 10.1021/jp303679yView Article
- Nguyen DT, Vedraine S, Cattin L, Torchio P, Morsli M, Flory F, Bernède JC: Effect of the thickness of the MoO3 layers on optical properties of MoO3/Ag/MoO3 multilayer structures. J Appl Phys 2012, 112: 063505. 10.1063/1.4751334View Article
- Wang HQ, Stubhan T, Osvet A, Litzov I, Brabec CJ: Up-conversion semiconducting MoO3:Yb/Er nanocomposites as buffer layer in organic solar cells. Sol Energy Mater Sol Cells 2012, 105: 196.View Article
- Barr MC, Howden RM, Lunt RR, Bulović V, Gleason KK: Top-illuminated organic photovoltaics on a variety of opaque substrates with vapor-printed poly(3,4-ethylenedioxythiophene) top electrodes and MoO3 buffer layer. Adv Energy Mater 2012, 2: 1404. 10.1002/aenm.201200112View Article
- Jung J, Kim DL, Oh SH, Kim HJ: Stability enhancement of organic solar cells with solution-processed nickel oxide thin films as hole transport layers. Sol Energy Mater Sol Cells 2012, 102: 103.View Article
- Wang ZY, Lee SH, Kim DH, Kim JH, Park JG: Effect of NiOx thin layer fabricated by oxygen-plasma treatment on polymer photovoltaic cell. Sol Energy Mater Sol Cells 2010, 94: 1591. 10.1016/j.solmat.2010.04.077View Article
- Steirer KX, Ndione PF, Widjonarko NE, Lloyd MT, Meyer J, Ratcliff EL, Kahn A, Armstrong NR, Curtis CJ, Ginley DS, Berry JJ, Olson DC: Enhanced efficiency in plastic solar cells via energy matched solution processed NiOx interlayers. Adv Energy Mater 2011, 1: 813. 10.1002/aenm.201100234View Article
- Ratcliff EL, Meyer J, Steirer KX, Garcia A, Berry JJ, Ginley DS, Olson DC, Kahn A, Armstrong NR: Evidence for near-surface NiOOH species in solution-processed NiOx selective interlayer materials: impact on energetics and the performance of polymer bulk heterojunction photovoltaics. Chem Mater 2011, 23: 4988. 10.1021/cm202296pView Article
- Ratcliff EL, Meyer J, Steirer KX, Armstrong NR, Olson D, Kahn A: Energy level alignment in PCDTBT:PC70BM solar cells: solution processed NiOx for improved hole collection and efficiency. Org Electron 2012, 13: 744. 10.1016/j.orgel.2012.01.022View Article
- Han S, Shin WS, Seo M, Gupta D, Moon SJ, Yoo S: Improving performance of organic solar cells using amorphous tungsten oxides as an interfacial buffer layer on transparent anodes. Org Electron 2009, 10: 791. 10.1016/j.orgel.2009.03.016View Article
- Vasilopoulou M, Palilis LC, Georgiadou DG, Argitis P, Kennou S, Kostis I, Papadimitropoulos G, Stathopoulos ΝΑ, Iliadis AA, Konofaos N, Davazoglou D, Sygellou L: Tungsten oxides as interfacial layers for improved performance in hybrid optoelectronic devices. Thin Sol Film 2011, 519: 5748. 10.1016/j.tsf.2010.12.207View Article
- Li N, Stubhan T, Luechinger NA, Halim SC, Matt GJ, Ameri T, Brabec CJ: Inverted structure organic photovoltaic devices employing a low temperature solution processed WO3 anode buffer layer. Org Electron 2012, 13: 2479. 10.1016/j.orgel.2012.06.045View Article
- Kim JR, Cho JM, Lee AR, Chae EA, Park JU, Byun WB, Lee SK, Lee JC, So WW, Yoo S, Moon SJ, Shin WS: Improvement of the performance of inverted polymer solar cells with a fluorine-doped tin oxide electrode. Curr Appl Phys 2011, 11: 175.View Article
- Ryu MS, Jang J: Enhanced efficiency of organic photovoltaic cells using solution-processed metal oxide as an anode buffer layer. Sol Energy Mater Sol Cells 2011, 95: 3015. 10.1016/j.solmat.2011.06.021View Article
- Li SS, Tu KH, Lin CC, Chen CW, Chowalla M: Solution-processable graphene oxide as an efficient hole transport layer in polymer solar cells. ACS Nano 2010, 4: 3169. 10.1021/nn100551jView Article
- Gao Y, Yip HL, Chen KS, O’Malley KM, Acton O, Sun Y, Ting G, Chen H, Jen AKY: Surface doping of conjugated polymers by graphene oxide and its application for organic electronic devices. Adv Mater 1903, 2011: 23.
- Han JT, Kim JS, Jo SB, Kim SH, Kim JS, Kang B, Jeong HJ, Jeong SY, Lee GW, Cho K: Graphene oxide as a multi-functional p-dopant of transparent single-walled carbon nanotube films for optoelectronic devices. Nanoscale 2012, 4: 7735. 10.1039/c2nr31923cView Article
- Wang Y, Liu J, Liu L, Sun DD: Enhancing stability and photocatalytic activity of ZnO nanoparticles by surface modification of graphene oxide. J Nanosci Nanotechnol 2012, 12: 3896. 10.1166/jnn.2012.6174View Article
- Notte LL, Salamandra L, Zampetti A, Brunetti F, Brown TM, Carlo AD, Reale A: Airbrush spray coating of amorphous titanium dioxide for inverted polymer solar cells. Int J Photoenergy 2012, 2012: 897595.View Article
- Peretz TS, Leman O, Nardes AM, Frey GL: On the origin of charge generation in hybrid TiOx/conjugated polymer photovoltaic devices. J Phys Chem C 2024, 2012: 116.
- Kong J, Lee J, Jeong Y, Kim M, Kang SO, Lee K: Biased internal potential distributions in a bulk-heterojunction organic solar cell incorporated with a TiOx interlayer. Appl Phys Lett 2012, 100: 213305. 10.1063/1.4722802View Article
- Ecker B, Egelhaaf HJ, Steim R, Parisi J, von Hauff E: Understanding s-shaped current–voltage characteristics in organic solar cells containing a TiOx interlayer with impedance spectroscopy and equivalent circuit analysis. J Phys Chem C 2012, 116: 16333. 10.1021/jp305206dView Article
- Shen L, Xu Y, Meng F, Li F, Ruan S, Chen W: Semitransparent polymer solar cells using V2O5/Ag/V2O5 as transparent anodes. Org Electron 2011, 12: 1223. 10.1016/j.orgel.2011.03.036View Article
- Yusoff ARBM, Kim HP, Jang J: Organic photovoltaics with V2O5 anode and ZnO nanoparticles cathode buffer layers. Org Electron 2012, 14: 858.View Article
- Stubhan T, Oh H, Pinna L, Krantz J, Litzov I, Brabec CJ: Inverted organic solar cells using a solution processed aluminum-doped zinc oxide buffer layer. Org Electron 2011, 12: 1539. 10.1016/j.orgel.2011.05.027View Article
- Chen TL, Betancur R, Ghosh DS, Martorell J, Pruneri V: Efficient polymer solar cell employing an oxidized Ni capped Al:ZnO anode without the need of additional hole-transporting-layer. Appl Phys Lett 2012, 100: 013310. 10.1063/1.3673843View Article
- Yusoff ARBM, Kim HP, Jang J: Comparison of organic photovoltaic with graphene oxide cathode and anode buffer layers. Org Electron 2012, 13: 2379. 10.1016/j.orgel.2012.07.024View Article
- Ghosh DS, Chen TL, Formica N, Hwang J, Bruder I, Pruneri V: High figure-of-merit Ag/Al:ZnO nano-thick transparent electrodes for indium-free flexible photovoltaics. Sol Energy Mater Sol Cells 2012, 107: 338.View Article
- Stubhan T, Krantz J, Li N, Guo F, Litzov I, Steidl M, Richter M, Matt GJ, Brabec CJ: High fill factor polymer solar cells comprising a transparent, low temperature solution processed doped metal oxide/metal nanowire composite electrode. Sol Energy Mater Sol Cells 2012, 107: 248.View Article
- Wang JC, Weng WT, Tsai MY, Lee MK, Horng SF, Perng TP, Kei CC, Yu CC, Meng HF: Highly efficient flexible inverted organic solar cells using atomic layer deposited ZnO as electron selective layer. J Mater Chem 2010, 20: 862. 10.1039/b921396aView Article
- Chemicool periodic table . Accessed 26 March 2014 http://www.chemicool.com/elements/lithium.html . Accessed 26 March 2014
- Jun BE, Kim YS, Park HJ, Kim SB, Yang HK, Park JH, Choi BC, Jeong JH: Effects of ambient oxygen pressures and substrate temperatures in pulsed laser deposited Zn0.85Li0.15O thin films. Thin Solid Films 2008, 516: 5266. 10.1016/j.tsf.2007.07.106View Article
- Lu JG, Zhang YZ, Ye ZZ, Zeng YJ, He HP, Zhu LP, Huang JY, Wang L, Yuan J, Zhao BH, Li XH: Control of p-and n-type conductivities in Li-doped ZnO thin films. Appl Phys Lett 2006, 89: 112113. 10.1063/1.2354034View Article
- Zeng YJ, Ye ZZ, Xu WZ, Li DY, Luand JG, Zhao BH: Dopant source choice for formation of p-type ZnO:Li acceptor. Appl Phys Lett 2006, 88: 062107. 10.1063/1.2172743View Article
- Li QH, Zhu D, Liu WJ, Liu Y, Ma XC: Optical properties of Al-doped ZnO thin films by ellipsometry. Appl Surf Sci 2008, 254: 2922. 10.1016/j.apsusc.2007.09.104View Article
- Wang XS, Wu ZC, Webb JF, Liu ZG: Ferroelectric and dielectric properties of Li-doped ZnO thin films prepared by pulsed laser deposition. Appl Phys A 2003, 77: 561.View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.